Acid-free hydrothermal process for synthesis of bioactive glasses 70SiO2-(30-x)CaO-xZnO (x=1, 3, 5 mol.%)

: Bioactive glasses 70SiO 2 -(30-x)CaO-xZnO (x=1, 3, 5 mol.%) were prepared by the acid-free hydrothermal method in keeping with the green chemical technology. The synthetic glasses were investigated by TG-DSC, BET, XRD, and SEM-EDX. All synthetic glasses present mesoporous structures consisting of aggregates of nano-particles. The bioactivity of synthetic glasses was confirmed through the formation of the hydroxyapatite phase after in vitro experiment in the SBF solution. The effect of Zn addition is shown through the decrease in the bioactivity of synthetic glasses. Additionally, the ICP-OES analysis indicates that the Zn ions were released from the glassy networks during in vitro experiments, and they act as Zn(OH) 2 suspended precipitation to inhibit the apatite deposition. The in vitro experiment in cell culture matter was performed for SaOS 2 and Eahy929 cells. The results confirmed the biocompatibility of synthetic glasses and the role of Zn addition in the proliferation of living cells.


Introduction
For the past five decades, bioactive glasses have been used as artificial bone materials thanks to their typical ability to connect to the natural bone by forming a hydroxyapatite layer during in vitro and in vivo experiments [1].These biomaterials can be synthesized by using two main methods melting and sol-gel [2].Recently, the sol-gel method has been widely applied because it has more advantages than the melting method.This method can produce bioactive glasses at moderate temperatures, preventing the final-product loss because of P2O5 evaporation.Furthermore, this method is able to synthesize bioactive glasses on nano-scale with mesoporous structures which reinforces the bioactivity of obtained materials [3][4].To control the bioactivity and biocompatibility of sol-gel glasses, beneficial elements such as Mg, Sr, Al, Cu, Fe, Ag, and Zn have been added [5][6][7][8][9][10][11].Among them, Zn plays an important role in bone formation because of its ability to inhibit the activity of osteoclasts and increase the differentiation of osteoblasts [12][13].Depending on the content of the doped Zn as well as the composition of the system, the synthetic glass systems exhibit different properties.Bioactive glass 64SiO2-26CaO-5P2O5-5ZnO (mol.%) has been elaborated by A. Balamurugan et al. using the sol-gel method.The authors pointed out that the incorporation of ZnO not only reduce the bioactivity of synthetic glass but also increase the osteoblast proliferation [6].Abeer M. El-Kady et al. have fabricated various sol-gel glasses 58SiO2-(33-x)CaO-9P2O5-xZnO (x = 1, 3, 5 wt.%) [14].All synthetic glasses exhibited high porosities, surface areas, and good bioactivity in the SBF test.Ternary 60SiO2-36CaO-4P2O5 (mol.%) and quaternary 60SiO2-25CaO-11Na2O-4P2O5 (mol.%)sol-gel glasses doped with 0, 1, 5 and 10 mol.% of ZnO have been synthesized by Julian Bejarano [15].The study indicated the content of doped ZnO influence on the textures, bioactivity, and compatibility of synthetic glasses.Furthermore, the increase of doped ZnO caused the decrease in formation of apatite mineral on glass surfaces after in vitro experiments.Thus, many glass systems containing ZnO have been studied by the sol-gel method.However, most synthesized ZnO-containing glasses used harmful strong acids and bases as catalysts for the hydrolysis process.In our previous study, the acid-free hydrothermal method has been used for synthesized binary bioactive glass with the molar composition of 70%SiO2-30%CaO [16].A combination of starting precursors without acid catalysts was heat-treated in a hydrothermal reactor at 150 oC for 24 hours.The obtained product in concentrated gel was dried and sintered at 700 oC during 3 hours.The synthetic glass was an amorphous structure and presented interesting bioactivity.Based on this approach, we synthesize the ternary bioactive glasses 70SiO2-(30-x)CaO-xZnO (mol.%,x=1, 3, and 5) within the present work.
The effects of ZnO additions on the physical-chemical properties, bioactivities, and biocompatibilities of synthetic bioactive glasses were investigated.

In vitro test in SBF solution
The bio-mineralization was verified by the immersion of bioactive glasses in the simulated body fluid (SBF) according to the method of Kokubo [17].The SBF synthetic solution has inorganic ion concentration similar to that of human blood.Glass powder samples with a mass of 125 mg were soaked in 250 mL of SBF at 37 oC with a stirring rate of 120 rpm for 1, 3, 5, and 7 days.At the end of each immersion phase, the powder samples are refined, dried, and used to determine their physical-chemical characterizations.The remaining solutions are served to measure the ionic concentration

In vitro test with cell culture
Two cell lines SaOS2 and Eahy929 were selected for culturing in DMEM (Dulbecco's Modified Eagle's Medium, Merck) at 37 oC in a humid environment (95% humidity, 5% CO2,) for 24 hours.The test ratio of glass sample/medium was chosen as 0.1 g/mL consistent with the ISO standard 10993-12:2007.The cell viabilities were determined by the MTT method following the previous report [18]

Physical-chemical characterization
The thermal analysis was performed by employing a Thermogravimetry-Differential Scanning Calorimetry (TG-DSC, Labsys Evo Setaram).The porous properties were determined from the nitrogen adsorption/desorption measurement on a micromeritics porosimeter (Quantachrome Instruments).The X-ray diffraction (XRD, D8-Advance) was served for phase identification.The morphology and elemental composition were investigated by using the Scanning Electron Microscopy (SEM) associated with the Energy Dispersive X-rays Spectroscopy (EDX) (SEM, S-4800, Japan).The ion behavior in SBF fluid was monitored by using the Inductively coupled plasma optical emission spectrometry (ICP-OES, ICP 2060).

Thermal behavior
Fig. 1 presents the TG-DSC curves of Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5.All glasses exhibited three mass-losses within the temperature ranges of 30-200, 200-400, and 400-600 oC.The primary mass-loss is characteristic for the removal of physically adsorbed water.This is shown on the DSC curves of the Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5 as the first endothermic peaks centered at 120.1, 127.9, and 142.6 oC, respectively [19].The second mass-loss with exothermic peaks concentrated at 313.1, 280, and 297.2 oC on the DSC curves of Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5, respectively, is due to the discharge of chemically adsorbed water [20].The third mass-loss with endothermic peaks centered at 535.4, 511.5, and 516.6 oC on the DSC curves of Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5, respectively, is related to the decomposition of nitrate groups [21].An exothermic peak without massloss at 963.6, 912.2, and 905.2 oC was observed on the DSC curves for Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5, respectively.This corresponds to the phase transition of the glass [21].The obtained result shows that the phase transion temperature decreased as the ZnO content in the glass increased.This demonstrates the effect of ZnO addition on the thermal properties of synthetic glasses as observed in the previous study [14].From the thermal analysis, the sintering temperature for synthesis of bioactive glasses was selected at 700 oC.

Phase analysis
XRD parternts of synthetic glasses Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5 are presented in Fig. 2. The obtained result indicated the amorphous nature of all synthetic glasses, no crystalline peaks were observed.As observed, the center of the diffraction halo was shifted to the right as the ZnO content increased from 1 to 5 mol.%.According to previous studies, Zn acts as Si to form up the glassy network, and can also replace Ca to act as a network modifier [14,22].Therefore, this phenomenon can be explained by the successful introduction of Zn2+ ions intertwined in the glass networks

Textural characterization
From the nitrogen adsorption/desorption mesuarement, the mesoporous properties of synthetic bioactive glasses were obtained as shown in the Tab.1.The obtained result indicates that the ZnO addition induced the reduction of porous structures of synthetic bioactive glasses.This is in line with the previous researches, where the authors showed that the incorporation of divalent ions such as Mg, Cu, Sr, or Zn significantly reduced the porous properties of synthetic glasses [23][24].The presence of Zn ions may disrupt the orderly association of the SiO4 tetrahedra within the self-assembly reaction, resulting in structural defects of the silica network, leading to the changes in mesoporous structures of synthetic bioactive glasses.3 represents the SEM-EDX analyses of synthetic bioactive glasses.Observing SEM images shows that Bioglass-Z1 exhibited a rough and porous surface while Bioglass-Z3, and Bioglass-Z5 had less porous surfaces.This observation is consistent with the above result obtained from the nitrogen adsorption/desorption analysis, confirming the effect of ZnO addition on the porous structure reduction of synthetic glasses.The EDX analyses confirmed the presence of the Zn element on the structure of synthetic bioactive glasses.

Bio-mineralization
Fig. 4 shows the XRD parents of bioactive glasses after immersion 5 days within the SBF solution.Two well-defined peaks at about 2θ=26o (002) and 32o (211) were observed for all glass samples.These characteristic peaks are contributed to the crystalline hydroxyapatite (HA) phase (JCPDS file No. 90432).This confirmed the bioactivity of all synthetic glasses.As increasing the ZnO contents, two characteristic peaks of HA showed less sharpness and lower intensity.The bioactivity of synthetic glasses can be arranged as Bioglass-Z1> Bioglass-Z3> Bioglass-Z5.This phenomenon is in line with the result achieved in previous research, confirming the effect of ZnO addition on the bioactivity of synthetic glasses [23,25].
The SEM micrographs including EDX analyses of bioactive glasses after 5 days of immersion within the SBF solution are shown in Fig. 5.The surfaces of all bioactive glasses were roofed by uniform, dense crystal layers.From the XRD analyses, this observation confirmed the hydroxyapatite formation on the surfaces of bioactive glasses after in vitro experiment.The HA layer on the surface of Bioglass-Z1 is more clearly defined than that of Bioglass-Z3, and Bioglass-Z5.The EDX analysis of glass samples after 5 days soaking in the SBF solution showed a sharp decrease in Si content because of the dissolution of the glass network.Meanwhile, Ca and P contents of soaked samples increased clearly, confirming the precipitation of Ca2+ and PO43-ions to create the apatite layer on the surface of bioactive glasses.The molar Ca/P ratios for the samples Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5 are 1.7, 2.2, and 2.8, respectively.The molar Ca/P ratio of hydroxyapatite (HA) is 1.67.Therefore, sample Bioglass-Z1 showed the best forming ability of HA layer compared to samples Bioglass-Z3 and Bioglass-Z5.Ionic changes within the SBF solution are associated with the physical-chemical reactions between the Zn-containing bioactive glasses and the physiological medium (Fig. 6).The initial SBF fluid contains 100 ppm of Ca, 0 ppm of Si, 31 ppm of P, and 0 ppm of Zn.After in vitro experiment, the ionicexchange behaviors are quite similar for all bioactive glasses.The Ca concentration increased and then decreased.The Si and Zn concentrations increased gradually while the P concentration decreased.The increase in Ca concentration is due to the rapid exchange between the Ca2+ ions of the glassy network and H+ ions in the physiological fluid [1].Subsequently, the Ca concentration plummeted to achieve saturation at 5 days of immersion.The decrease in Ca concentration is expounded to its consumption to form the mineral HA on the surface of bioactive glasses [1-2].As well as the decrease of Ca concentration, the P concentration was noted to decrease because of its consumption to form the apatite mineral layer [1-2].It can be seen that the consumption of Ca and P to form the HA layer of Bioglass-Z1 is the most, followed by Bioglass-Z3, and Bioglass-Z3.The Si concentration increased rapidly on the first day of soaking, then moderately increased to succeed in saturation at 5 days.The increase in Si concentration is explained by the solubility of the glassy network through the discharge of Si(OH)4 acids while the saturation process corresponds to the self-assembly reactions of the above acids to form the silica SiO2 layer [1-3].The amount of Zn released increased within the order Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5, in keeping with the content of ZnO added to the synthetic glasses.According to the literature [23,26], a component of the Zn ions released will form the Zn(OH)2 precipitation, which prevents the deposition of HA on the glass surfaces.This is suitable when the precipitation of HA decreases as the concentration of added ZnO increases in synthetic glasses.

Bio-compatibility
Figure 7 shows the cell viability of the SaOS2 and Eahy929 lines when exposed to the bioactive glasses for 24 hours.Cell viability without glass contact was chosen as the control (100%) [18].
According to the ISO standard 10993-5 (in vitro test for cytotoxicity), cell viability is set as a percentage relative to the control.if the cell viability is a smaller amount than 70%, the material is cytotoxic.Therefore, all synthetic bioactive glasses (Bioglass-Z1, Bioglass-Z3, and Bioglass-Z5) have good biocompatibility.The Bioglass-Z5 exhibits the foremost effective biocompatibility compared with the samples Bioglass-Z3, and Bioglass-Z1.The obtained results are consistent with previous studies, confirming the effect of ZnO addition on the enhancement of cell viabilities [14][15].

Conclusion
The study confirmed that the acid-free hydrothermal process was suitable for the synthesis of the bioactive glasses 70SiO2-(30-x)CaO-xZnO (mol.%,x = 1, 3, 5).All synthetic glasses have an amorphous nature.The bioactivity of synthetic glasses was confirmed by the formation of a new layer of hydroxyapatite mineral on the surface of the glass samples after in vitro test in SBF liquid.The effectiveness of the ZnO addition was shown by inhibiting the bioactivity of synthetic glasses.In vitro test within the cellular medium has confirmed the good biocompatibility of the synthetic glasses and also the positive effect of ZnO addition on cell viability.

Table 1 .
Values of specific surface area, pore diameter, and pore volume for synthetic glasses.